Standard Practice for Preparing Test Specimens From Basic Refractory Gunning Products by Pressing
Five brick specimens are prepared using the water content specified by the manufacturer. This procedure assures the preparation of uniform specimens for testing purposes. At least 50 lbs. of each material for testing should be submitted. Mixing is performed in a Hobart mixer and specimens are formed at 1800 psi.
SIGNIFICANCE AND USE
This practice defines a procedure that ensures consistent preparation of specimens for product testing and evaluation.
This practice can be used in the laboratories of producers, users, and general-interest parties for research and development or quality-control work. It is particularly useful for interlaboratory comparisons on products, for repetitive evaluations or comparisons of products or product equality, and in specifying a uniform preparation practice for specimens for acceptance testing.
In using this practice, it must be recognized that the structure of laboratory-pressed specimens may differ significantly from the structure of material gunned in field applications.
1.1 This practice covers a procedure for preparing test specimens from basic refractory gunning products by pressing prepared material in a mold. After pressing, test specimens prepared from dolomitic mixes are subjected to a prescribed heat treatment. Specimens prepared in accordance with this procedure are intended for use in ASTM test methods.
1.2 The values stated in inch-pound units are to be regarded as standard. The values given in parentheses are mathematical conversions to SI units that are provided for information only and are not considered standard.
1.3 This standard does not purport to address all of the safety problems, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
Extracted, with permission, from ASTM C973 Standard Practice for Preparing Test Specimens From Basic Refractory Gunning Products by Pressing, copyright ASTM International, 100 Barr Harbor Drive, West Conshohocken, PA 19428. A copy of the standard may be purchased from ASTM International, phone 610-832-9555, e-mail: firstname.lastname@example.org, website: www.astm.org.
FROM THE BLOG...
01/18/2019New Laboratory Training Course Announced
LABORATORY TRAINING - THERMAL PROPERTIES OF REFRACTORIES - March 19, 20 & 21, 2019 A Three Day Course...
ADVANCED THERMAL PROPERTIES OF REFRACTORIES - October 29 & 30, 2018 A Two Day Course Sponsored by...
In response to industry demand, Orton is offering a series of new short courses dealing with refractories...